Fire performance of recycled rubber-filled high-strength concrete
Cement and Concrete Research 34 (2004) 109 – 117 Fire performance of recycled rubber-filled high-strength concrete F. Hernandez-Olivaresa, G. Barluengab,* ´ a ´n ´ ´ ´ ´ Departamento de Construccio y Tecnologıa Arquitectonicas, Escuela Tecnica Superior de Arquitectura, Universidad Politecnica de Madrid, Avda. Juan de Herrera, 4, 28040 Madrid, Spain b ´ ´ ´ ´ Departamento de Tecnologıa de la Edificacion, Escuela Universitaria de Arquitectura Tecnica, Universidad Politecnica de Madrid, Avda. Juan de Herrera, 6, 28040 Madrid, Spain Received 19 November 2002; accepted 16 July 2003Abstract The paper presents the behavior of a high-strength concrete (HSC) with silica fume (SF) modified with different amounts of solid particlesrecycled from crumbed used truck tires. The aims of including elastomeric materials in a cementitious matrix are reducing the stiffness ofHSC in order to make it compatible with other materials and elements of the building, unexpected displacement of foundations andshrinkage, recycling of solid wastes and improving fire performance. The inclusion of low volumetric fractions of rubber reduces the risk of explosive spalling of HSC at high temperatures because watervapor can exit through the channels left as the polymeric particles get burnt. The temperature reached at a fixed depth of the fire-testedspecimens is reduced as the percentage of rubber increase. A set of mechanical, destructive and nondestructive tests were accomplished in order to obtain optimum quantities of crumbed used tiresrubber in the composition, taking into account workability, stiffness and, obviously, strength. The results obtained show that a relatively high-volume fraction of rubber (3%) does not reduce significantly the strength, although it reduces the stiffness. Higher values of rubber produce aprogressive reduction of strength and stiffness but might improve the dynamic behavior.D 2003 Elsevier Ltd. All rights reserved.Keywords: Mechanical properties; Waste management; Fire performance; Rubber-filled high-strength concrete1. Introduction HSC presents another important difference with regard to NSC. Recent HSC fire tests results have shown that there High-strength concrete (HSC) is a new material that can are well-defined differences between HSC and NSC prop-now be manufactured by most concrete plants. The avail- erties at high temperatures . HSC shows a higher ten-ability of a variety of additives such as silica fume (SF) and dency of explosive spalling when subjected to rapid heating,water-reducing admixtures (WRA) allows its widespread as in the case of fire [2– 4]. This behavior is mainly due touse. In terms of architectural advantage, HSC allows smaller the lower permeability that results in a build-up of poresize columns to be used in high-rise buildings, which results pressure within the cement paste . Some solutions, as thein more usable space in the lower floors. inclusion of polypropylene fibers to allow the water vapor Further than strength, HSC has significant differences escape from the concrete matrix, have been proposed towith regard to normal strength concrete (NSC). Higher reduce the risk of spalling [6,7].stiffness, lower permeability and larger durability are This paper presents some results of an experimentalsome of these differences. For this reason, some struc- program on HSC filled with solid fiber-shaped particles oftural codes do not cover the use of this material or recycled tire rubber performed at the Materials Laboratorypresent special recommendations for its use as structural of the School of Architecture of Madrid. The objectives ofmaterial . this study are as follows: Reduce the risk of HSC explosive spalling when fire * Corresponding author. Tel.: +34-91-336-7612; fax: +34-91-336- occurs. Management of solid wastes from used truck tires,7637. E-mail address: firstname.lastname@example.org (G. Barluenga). reducing environmental impact.0008-8846/$ – see front matter D 2003 Elsevier Ltd. All rights reserved.doi:10.1016/S0008-8846(03)00253-9
110 ´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117Table 1 evolution of the hardening process. Compression tests wereNominal properties of truck tire rubber also made at different ages to measure the increase ofYoung modulus strength along time.@ 100% 1.97 MPa Prismatic nonstandard specimens (20 Â 30 Â 5 cm) of all@ 300% 10 MPa compositions were manufactured for fire performance tests.@ 500% 22.36 MPa The equipment used for performing the fire tests wasTension strength 28.1 MPaBreak point strain 590% composed by the following:Resilience Furnace CHESA, technical data:@ 23 jC 44% – Six gradual electric resistance@ 75 jC 55% – Maximum temperature of 1300 jC. – Dimensions of fire hole of 15 Â 30 cm. – Register of furnace temperature with a type S Reduce the HSC stiffness without a high loss of strength, thermocouple. enlarging the compatibility of deformation with other – Furnace controller CHESA, with 6 different temper- building elements. ature programs. Two type K thermocouple in contact with both internal Some research has been done concerning with rubber- and external faces, respectively. Temperature transducers Testo 925 for type K thermo-filled NSC (also called rubberized concrete) [8 – 14], al-though rubber-filled HSC has not been previously described. couples. Thermogravimetric tests were carried out with pattern2. Experimental program samples and samples extracted from several depths of the fire-tested specimens in order to obtain damage spectrums A base HSC composition with SF and without fiber was of the rubber-filled HSC compositions under study. Withdetermined. Then three different rubber fiber volumetric this test, the temperature reached at each distance can befractions (3%, 5% and 8%, respectively) were included to found out, comparing the weight loss of the sample whenthe base composition. heated at a certain temperature with a pattern sample. The rheological behavior of the material in fresh statewas measured using the slump and the Ve-Be consistometertests. 3. Materials In the hardened state, porosity and density were mea-sured. Sets of six cubic specimens (10 cm) of each compo- Four compositions of HSC filled with different smallsition were manufactured. Ultrasonic pulse nondestructive volumetric fractions of solid fiber-shaped particles oftests were performed at several ages in order to measure the recycled tire rubber (0%, 3%, 5% and 8%) were used. Fig. 1. Ultrasonic modulus of several compositions at different ages of rubber-filled HSC.
´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117 111 Fig. 2. Compressive strength of different compositions at different ages of rubber-filled HSC. The base HSC composition is described next (dosage for Relation coarse aggregate/cement = 2.1/11 m3) : Relation fine aggregate/cement = 1.33/1 Cement type CEM I—52.5 R (Asland)—513 kg The rubber fiber is included to this composition in 3%, Rolling siliceous coarse aggregate (maximum size of 16 5% and 8% volumetric fractions (25.2, 42 and 67.2 kg/m3, mm)—1080 kg respectively). Siliceous fine aggregate (maximum size of 4 mm)—685 The solid fiber-shaped particles of recycled tire rubber kg come from truck tires wasted away after a second recapping. SF (5% of weight with respect to cement)—25.65 kg The length of the fibers is between 0.85 and 2.15 cm, with Superplasticizer Glenium C-355 (Bettor-MBT) (3% of an average value of 1.25 cm. Its surface is rough and quite weight with respect to cement)—15.7 kg damaged due to the cut process. It contains 4% of dust Water—128.25 l particles that act as air entraining admixture. Its density is Relation water to cement (w/c) = 0.25 0.84 g/cm3 and a water absorption rate of 25% has been Fig. 3. Relation between compressive strength and density at different ages of rubber-filled HSC.
112 ´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117 Fig. 4. Relation between ultrasonic modulus and compressive strength at different ages of rubber-filled HSC.measured. A softening temperature of 175 jC and a com- min. At last, water and superplasticizer were added and thebustion temperature of 200 jC have been determined. process continued for 15 min. Table 1 presents other nominal properties of tire rubber All the slump tests results were larger than 10 cm and. the values of time obtained with the Ve-Be tests shorter than 15 s. The Ve-Be time increased as the percentage of rubber increase, although all the compositions had a usable4. Mixing procedure and rheological behavior workability. The HSC compositions were mixed using a 50-l horizon-tal axis mixer. The low w/c ratio used (0.25) and the 5. Physical and mechanical characterization resultsinclusion of SF forced to change the mixing process withregard to NSC. The coarse aggregate, the cement, the rubber One set of six cubic specimens (10 cm) and twofibers and the SF were mixed first for 2 min. Then the fine cylindrical specimens (F15 Â 30 cm) per compositionaggregate was included, continuing the mixing process for 1 under study (0, 3, 5 and 8 vol.% rubber fiber-filled HSC) Fig. 5. Fire tests results of rubber-filled HSC specimens without rubber.
´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117 113 Fig. 6. Fire test results of rubber-filled HSC specimens with 3% volumetric fraction of rubber.were manufactured. The specimens were produced with be observed that the higher the amount of rubber, the lowersteel molds, vibrated the time obtained in the Ve-Be tests, the ultrasonic modulus and therefore the stiffness.in order to avoid segregation of the mixture. The external Cubic specimens were used for compression tests. Inface of the specimens was watered in order to avoid order to avoid stress concentrations on the contact sides ofsuperficial drying up. The specimens were demolded 24 the specimens, which can produce the failure of the spec-h after filled and they were water cured. The specimens imen at lower strength than normal, 1-cm thick distributionwere taken out of the water several hours before tested to steel plates were used.allow drying. Ultrasonic pulse tests were performed on all Compression test results are summarized in Fig. 2. It canthe specimens before testing. The results of ultrasonic be remarked that the compressive strength decreases withmodulus were obtained with the equation (Eq. 1), the increase of the amount of rubber fiber. Although for small volumetric fractions of rubber, the decrease is quite reduced. The failure of HSC specimens without rubberEs ¼ qv2 =1000 ð1Þ occurred in an explosive manner. The specimens with rubber did not show explosive failure.where Es is the ultrasonic modulus (MPa), q is the density It can be observed that the shape of the curve that(g/cm3) and m is the velocity of ultrasonic pulse propagation represent the evolution of the strength with age changes(m/s). Results are summarized in Fig. 1. when rubber fiber is included. The ultrasonic modulus is a good index of the stiffness of Fig. 3 relates the compressive strength and the densitythe material and is useful as a comparison value . It can measured at different ages. Fig. 4 relates ultrasonic modulus Fig. 7. Fire test results of rubber-filled HSC specimens with 5% volumetric fraction of rubber.
114 ´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117 Fig. 8. Fire test results of rubber-filled HSC specimens with 8% volumetric fraction of rubber.with compressive strength at different ages. Both relations performed until the exposed side of the specimens reachedfit with a linear approximation. 1000 jC. The experimental results of the fire tests are summarized in Figs. 5 – 8. The specimens tested shown a very different behavior.6. Fire performance of HSC filled with recycled tire The specimen of HSC without rubber fiber presentedrubber spalling on the exposed side and a very remarkable curva- ture. Fig. 9 shows the surface exposed to fire of the The study of the behavior of HSC filled with solid specimen with 0% of rubber fiber after the fire test. Thefiber-shaped particles of recycled tire rubber under fire specimens with rubber fiber did not show spalling and theincluded a fire test following EN-UNE 1363-1 (equivalent curvature of the plate was lower as the volumetric fractionto ISO 834) . The equation used for the fire curve was of rubber increased. Fig. 10 shows the exposed surface of(Eq. 2), the specimen with 3% of rubber, and Fig. 11 presents a comparison of the curvatures occurred to the specimens dueT À T0 ¼ 345 log10 ð8t þ 1Þ ð2Þ to fire effect. The curvature measured after fire tests on the tested specimens is represented in Fig. 12. A linear relationwhere T is the temperature at the time t and T0 is the between percentage of rubber and radius of curvature hastemperature at the beginning of the test. been observed. Prismatic specimens (20 Â 30 Â 5 cm) of all composi- Thermogravimetric tests were performed on samplestions under study (0%, 3%, 5% and 8% rubber fiber extracted from the fire-tested specimens at different distan-volumetric fraction content) were tested. The tests were ces from the exposed surface. Samples extracted from theFig. 9. Exposed surface of rubber-filled HSC specimen with 0% of rubber Fig. 10. Exposed surface of rubber-filled HSC specimen with 3% of rubberafter fire test. General view and detail. after fire test. General view and detail.
´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117 115Fig. 11. Lateral view of the fire-tested rubber-filled HSC specimens with Fig. 13. Thermogravimetric test results of pattern samples extracted fromdifferent percentages of rubber. untested rubber-filled HSC specimens with different percentages of rubber.specimens subjected to compression tests were also tested inorder to obtain a pattern to compare with. Fig. 13 summa- workability. The combination of static (slump test) andrizes the results obtained from thermogravimetric tests of dynamic (Ve-Be test) workability tests gave a knowledgethe pattern samples. of the rheological behavior of the rubber-filled HSC. The The samples extracted from the plates that were inclusion of SF and rubber in the composition can maintainsubjected to fire tests were obtained from 1, 2, 3 and a good slump, but the Ve-Be times varied. The Ve-Be test4 cm depth. The samples were heated at temperatures gave information about the vibration time necessary tofrom 0 to 900 jC, on intervals of 100 jC, and weighted compact the material without segregation.after each stage. The results of weight loss were com- In the hardened state, a significant relation amongpared with the pattern samples to determine the temper- density, ultrasonic modulus and compression strength hasature reached at each depth in the fire test. Fig. 14 been observed, as shown in Figs. 3 and 4. As rubber density,summarizes the results obtained from the thermogravi- compressive strength and stiffness are lower than HSCmetric tests. It can be observed that the higher the rubber properties, the more rubber has the composition, the lowerfiber content, the lower the temperature reached at the is the density, the compressive strength and the stiffness ofsame depth. the rubber-filled HSC. For low volumetric fractions of rubber fiber (3%), the reduction of strength is around 10%.7. Discussion of results The inclusion of rubber fiber eliminates explosive failure of HSC under compression. Rubber fibers main- The workability of the rubber-filled HSC decreased with tained the sides of the cracks together and the failure wasthe increase of rubber fiber, though it remained good progressive. Fire performance of HSC changes when rubber is in- cluded in the composition. Explosive spalling occurred in HSC without rubber, as shown in Fig. 9. The curve of external surface temperature (unexposed to fire) presented a step when spalling happened (Fig. 5). The open channels left when rubber particles get burnt allows the water vapor escape from the sample, reducing stress due to vapor pressure. Small holes can be observed in the fire-exposed surface of the specimens with rubber fiber (Fig. 10). No holes are present on the specimen without rubber (Fig. 9). There is a linear relation between percentage of rubber and the radius of curvature measured on the fire-tested specimens. The curvature observed on the fire-tested speci- mens is produced by thermal gradient and vapor pressure.Fig. 12. Curvature of the fire-tested rubber-filled HSC specimens with The more rubber in de composition of HSC, the larger thedifferent percentages of rubber. curvature, as can be observed in Fig. 11.
116 ´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117Fig. 14. Temperature reached at different distances from the exposed surface of the fire-tested rubber-filled HSC specimens with different percentages of rubber. Thermogravimetric test results point out a decrease of Acknowledgementsthe temperature reached at a certain distance from theexposed surface when the amount of rubber increases. The authors want to acknowledge the collaboration in theConsidering 500 jC as the temperature when steel rein- specimens preparation and testing of the students of Archi-forcement loses its mechanical capacity, a depth of damage ´ tecture Irene Herrera, Juan A. Soria and Laura Fernandez.can be defined on rubber-filled HSC. At larger distancesfrom the exposed surface, the structural integrity can beexpected. References Fig. 14 shows that a column of HSC without rubberwould need a larger reinforcement covering than other made  CEN, Eurocode 2: Design of Concrete Structures: Part 1 – 2. Structuralof rubber-filled HSC in order to guarantee structural integ- fire design, CEN/TC 250/SC, 1993.rity. Explosive spalling of HSC has to be taken into account  L.T. Phan, Fire performance of HSC: a report of the state of the art, NISTIR 5934, NIST, 1996.too, as previously mentioned.  Y. Anderberg, Spalling phenomena of HPC and OC, Proceedings of the International Workshop on Fire Performance of High-Strength Concrete, NIST, Gaithersburg, 1997.8. Conclusions  L.T. Phan, J.R. Lawson, F.L. Davis, Heating, spalling and residual properties of high performance concrete, NISTIR 6588, NIST, 2000. Rubber-filled HSC shows a decrease of compressive  P. Kalifa, F. Manneteau, D. Quenard, Spalling and pore pressure instrength and stiffness, with regard to HSC, when the HPC at high temperatures, Cem. Concr. Res. 30 (2000) 1915 – 1927.percentage of rubber in its composition increases. This  P. Kalifa, G. Chene, C. Galle, High-temperature behaviour of HPCbehavior can be profitable when some ductility of the with polypropylene fibers. From spalling to microstructure, Cem.material is required, maintaining high strength. HSC filled Concr. Res. 31 (2001) 1487 – 1499.  D.P. Bentz, Fibers, percolation and spalling of HPC, ACI Mater. J. 97with 3% volumetric fraction of rubber present a reduction of (3) (2000) 351 – 359.mechanical characteristics of only 10%.  N. Segre, I. Joekes, Use of tire rubber particles as addition to concrete The fire tests have shown a reduction of curvature and paste, Cem. Concr. Res. 30 (2000) 1421 – 1425.risk of explosive spalling when HSC is filled with rubber.  Z.K. Khatib, F.M. Bayomy, Rubberized Portland cement concrete,The depth of damage (temperature over 500 jC for rein- J. Mater. Civ. Eng. 11 (3) (1999) 206 – 213.  I.B. Topcu, Analysis of rubberized concrete as a composite material, ßforced concrete structures) is also reduced. This could mean Cem. Concr. Res. 27 (8) (1997) 177 – 183.a reduction of the reinforcement covering in structural  D. Raghavan, H. Huynh, C.F. Ferraris, Workability, mechanical prop-elements or an increase of safety in HSC structural elements erties and chemical stability of a recycled tyre rubber-filled cementi-against fire. tious composite, J. Mater. Sci. 33 (1998) 1475 – 1752.  I.B. Topcu, Assessment of the brittleness index of rubberized concrete, ß More research is needed to develop this material though Cem. Concr. Res. 27 (2) (1997) 1135 – 1139.the results obtained show a good behavior in general terms.  I.B. Topcu, Collision behaviours of rubberized concrete, Cem. Concr. ßThe management of solid waste is also a goal of this Res. 27 (12) (1997) 1893 – 1898.material. ´  F. Hernandez-Olivares, G. Barluenga, M. Bollati, B. Witoszek, Static
´ F. Hernandez-Olivares, G. Barluenga / Cement and Concrete Research 34 (2004) 109–117 117 and dynamic behaviour of recycled tyre rubber-filled concrete, Cem.  W.H.Y. Waddell, L.R. Evans, Use of non-black fillers in tire com- Concr. Res. 32 (2002) 1587 – 1596. pounds, Rubber Chem. Technol. 69 (3) (1996) 377. ´ ´ ` P.-C. Aıtcin, Le developpement des betons a hautes performances en ¨  J.C. Wang, Young’s modulus of porous materials, J. Mater. Sci. 19 ´ ´ ` Amerique du Nord, in Les betons a hautes performances. Caracterisa-´ (1984) 809 – 814. ´ ´ tion, durabilite, applications, Presses de l’ecole nationale des Ponts et  UNE-EN 1363-1, Ensayos de resistencia al fuego: Parte 1. Requisitos ´ chaussees, Paris, 1992. generales.